4.3 IR microscopy
5.1.1 Current-voltage characteristic
The CZT samples are prepared as described in the Cutting and polishing sec-tion, following a careful procedure for the preparation of an optimal surface.
The removal of the damaged parts after the cutting is very important and strongly inuences the detector properties. The damaged layers in fact contain a high concentration of inclusions that can results in a deformation of the elec-tric eld. The surface roughness represents as well a critical parameter in the realization of good radiation detectors . The presence of residual impuri-ties, mostly due to the polishing procedures, on the surface before the contact deposition can lead to the formation of an interlayer between the metal contact and the CZT. This layer strongly alters the characteristic of the contact. How-ever this problem can be easily avoided by cleaning the samples with sHow-everal baths in organic boiling solvents, like acetone, isopropanol and trichloroethy-lene. The Br-methanol etch removes all the possible residual on the surface and the native oxide, but it's well known to produce a Te rich surface that rapidly oxidize in air. The resulting oxide is more conductive with respect to the bulk CZT and hence the drawbacks of this procedure must be taken into account   . A bad polishing can also aect the contact properties, a rough surface origins a bad adhesion of the metal to the CZT surface. The polishing procedure used at IMEM produces a good surface. As conrmed by the AFM measurement the roughness is conned in the range ≤ 1nm. The study of the
-300 -200 -100 0 100 200 300 -1,5x10-8
-1,0x10-8 -5,0x10-9 0,0 5,0x10-9 1,0x10-8 1,5x10-8 2,0x10-8
-300 -200 -100 0 100 200 300
-6,0x10-9 -4,0x10-9 -2,0x10-9 0,0 2,0x10-9 4,0x10-9 6,0x10-9 8,0x10-9 1,0x10-8
Figure 5.1: The two typical behavior found in the IMEM CZT samples. In a) the increasing resistance behavior, at low voltages the resistance value is lower and then increase for high voltages. b) The resistance decrease with the increase of the applied bias
contact properties was the aim of my master degree and represent an accurate analysis of the eect of the surface preparation and the passivation process on the IV characteristics of the Au evaporated contact . The contact de-position techniques available at IMEM are the thermal evaporation and the electroless technique. The electroless deposition is a very quick way to deposit a metal on the surface of the semiconductor and produces a very good current voltage characteristic with low surface leakage currents. The used solution was a 4% AuCl3 water solution, as reported in (insert citation)the optimal depo-sition time for the Au solution is 1 minute, after that time the reaction does not evolves and the total amount of metal is deposited. The current voltage characteristics as reported in  are directly connected with the spectral res-olution of the devices, and in particular the behavior at high bias. The author classies three dierent curves: the increasing resistance, the linear behavior and the decreasing resistance. The optimal curve for the spectral response was found to be the increasing resistance. For the IMEM samples only two kind of curves were found: the increasing and the decreasing resistance 5.1. The two behaviors corresponds to a completely dierent response in the presence of the X-ray sources.
A clear example of the importance of the IV characteristics on the detector performance is shown in gure 5.2. The image shows the two IV characteristics and the corresponding spectroscopic response of two sample irradiated with an
241Am X-ray source.
The two samples were cut from the same wafer, of the same crystals en-suring the higher possible similarity between the crystal properties of the two samples. Also the thickness (2mm) and the dimensions (7 x 7 mm2) are the same. The two samples dier in the IV characteristics, sample 024-04-d shows
-200 -100 0 100 200 300 -8,0x10-9
-6,0x10-9 -4,0x10-9 -2,0x10-9 0,0 2,0x10-9 4,0x10-9 6,0x10-9 8,0x10-9 1,0x10-8
Voltage (V) 024-04-b 024-04-d
0 50 100 150
0 1000 2000 3000 4000
Energy (keV) Am241
0 50 100 150
0 2000 4000 6000 8000
Figure 5.2: The dierent spectroscopic response and the corresponding IV character-istics of two CZT samples cut from the same wafer, they have the same thickness and the same surface area. The IV curve with an increasing resistivity shape shows a very good 241Am spectrum, while the sample with the decreasing resistivity characteristic has a bad response. It is important to underline that the current value itself is not a signicant parameter for the determining of the good functioning of the device, in fact in this case the current value is similar.
the increasing resistivity curve, sample 024-04-b the decreasing resistivity one.
The same contact deposition technique was used for both the samples: electro-less gold, for 1 minute on each side. The two IV curves do not dier much in terms of the current owing in the devices, in fact for negative biases the 024-04-d sample shows higher current with respect to 024-04-b. The positive slope has instead the opposite behavior, in both cases, anyway, the current value are comparable. The main dierent consists in the curve shape, for 024-04-b the current voltage curve has an exponential increase at high voltages (above 150V), the 024-04-d shape is instead showing the characteristic linear charac-teristic in the high voltage region. The trend showed in 024-04-b to increase exponentially the currents owing in the device is enhanced in presence of the radiation source, and hence when the charge carriers are generated, leading to a strong contribution of the noise in the device, as shown in the241Am spectrum.
Since any other characteristic of the device seem to similar (the µτ products are almost identical, the Te inclusion density are similar and the Zn concentra-tion is the same since the sample are cut from the same posiconcentra-tion in the growth axis) the main dierences are ascribed to the IV curves. This dramatic change in the current voltage behavior may be due to the dierent surface condition, related to a non reproducibility of the eectiveness of the cleaning procedure or to a dierent eld distribution. The study of the contacts by means of the RBS and XRF techniques (illustrated in the next section) highlighted a much higher damage in the case of the 024-04-b with respect to the 024-04-d: the thickness of the layers with a dierent stoichiometry with respect to the bulk is almost three time higher in sample 024-04-b. This measurement shows one of the main limits of the electroless technique, the poor reproducibility in the contact characteristics .
RBS and XRF analyses
The two deposition techniques, thermal evaporation and electroless deposition of gold, were studied using the combination of two techniques: Rutherford Backscattering (RBS) and X-ray uorescence. The measurements were per-formed by Dr. A. Raulo at the University of Napoli Federico II. The recorded spectra were analyzed using the SIMNRA 4.4 software package. The study pointed out two dierent behaviors for the deposition techniques. The thermal evaporation aects a small region under the metal contacts, usually conned in a region up to 1500 Å, this region presents a deviation from the bulk com-position mostly due to the creation of an oxidized region near the surface. For the electroless deposition technique the behavior is completely dierent. In this case several layers can be identied by the software modeling. As reported
Figure 5.3: RBS spectrum of a CZT sample with thermal evaporated gold contacts
in  during the reaction with chloride the Cd ions leave the materials and pass in the solution, the metal ions, in this case Au, deposits on the surface creating the electrode. The electroless process leaves a layer near the surface with a decreased Cd concentration, due to the migration of the ions, and the typical Cd vacancies. The stoichiometry of the rst layers is strongly deviated from the bulk one, the presence of various oxide layer was also identied in the study. The total damaged layer, that comprehends all the dierent layers that do not present the stoichiometry of the bulk, is much higher for the electroless contacts.
The deposited metal layer is thicker then the expected value from the lit-erature , and shows a maximum value of 70 nm for the Cd terminating surface. The reaction is favorite by the excess of Cd due to the orientation of the  oriented surface and consequently the deposition is higher on one of the two surfaces. In  are also studied the Pt electroless contacts, the metal deposited layer is much thinner for the Pt chloride solution, only 10 nm, even if the deposition times were 4 minutes and 10 minutes. The I-V characteristics are dominated by the surface conductive paths generated after the deposition and the resulting currents are very high. The passivation of the surface was found to be ineective, the current level after the passivation process is still very high. It is hence impossible to use such contact solution for the realization of radiation detector devices.
Figure 5.4: IV curve showing the two slopes for low and high applied voltages. b) low voltage region, the contribution of the bulk is highlighted by the blue line